Influences of atmospheric water vapor on spectral effective emissivity of a single-layer radiative cooling coating

: Radiative cooling technology can emit infrared heat to the outer space through the “sky window” for cooling without consuming energy, which had drawn more and more attention. However, some researches reported that there was a significantly different cooling performance at different atmospheric total water vapor columns (TWC) conditions. In this study, taking a simple single-layer radiative cooling coating containing two kinds of particle mixture (SiO 2 , TiO 2 ) as example, the spectral effective emissivity of the radiative cooling coating was proposed to evaluate the effect of the atmospheric water vapor on the cooling performance. The spectral effective emissivity of the coating was obtained through multiplying spectral emissivity of the coating by the atmospheric transmittivity, where the spectral emissivity was calculated by combining an algorithm for calculating radiative properties of the multi-particle system with the Monte Carlo ray-tracing method (MCRT). The effects of different atmospheric water vapor on the spectral effective emissivity of the simple single-layer radiative cooling coating containing different particles size, volume fraction and thickness were studied to improve the cooling performance of the coating. The results


Introduction
With the energy crisis and global warming, human beings were paying more attention to energy saving and emission reduction technology [1][2][3][4].The building refrigeration system consumed approximately 20% of the global indoor electricity and accounted for 10% of the global greenhouse gas emissions [5,6].The energy consumption of the air conditioner could be reduced by 3-5% for every 1 ℃ reduction of the temperature needed to be reduced.The daytime radiative cooling technology can reflect sun irradiation strongly and emitted infrared energy to the outer space through 'sky window', which could achieve several degrees of cooling below ambient temperature without consuming any additional energy [7][8][9].This technology has very broad prospects, which could be applied in the fields of constructions, refrigerated vehicles and photovoltaic cells [10,11].Radiative cooling technology had attracted many researchers to prepare high-performance radiative coolers [12][13][14].
In recent years, in order to obtain high-performance radiative cooling materials, researchers had done a lot of work on the design and preparation of films, nanoparticle-based coatings and photonic structure devices [15][16][17][18][19][20].For example, Raman et al.21 prepared a multi-layer photonic radiative cooler by magnetron sputtering HfO 2 and SiO 2 .This radiative cooler achieved a cooling power of 40 W/m 2 and a sub-ambient temperature drops of nearly 5 ℃ under solar irradiation.Fan et al. proposed a radiative cooling foil composed of a fluorinated polyimide embedding SiO 2 microspheres.This radiative cooling foil achieved a cooling effect of 4.6 ℃ lower than ambient temperature.Cheng et al. 22 proposed a single-layer radiative cooling coating that the reflectivity (0.3-2.5 μm) and the emissivity (8.0-13.0μm) were more than 0.95.Huang et al. 23 designed a double-layer radiative cooling coating that the top layer embedded with TiO 2 particles reflected 90% of solar irradiation and the bottom layer embedded with carbon black particles emitted 90% of infrared heat to the outer space.
The researchers designed high-performance radiative cooling materials, but the same material had a significantly different cooling performance when they were tested at different regions or weather conditions.Atmospheric water vapor was regarded as the most important factor affecting cooling performance of radiative cooling materials [23][24][25][26][27]. Zhai et al. 28 invented metamaterial containing glass particles for radiative cooling.This metamaterial could reflect 96% of solar radiation and had a 93% average emittance in the 'sky window' region.The cooling power was 93 W/m 2 during daytime in Arizona on the dry autumn days (October [16][17][18][19].However, Ref. 29 which was published from the research group of Zhai et al. reported that daytime cooling power of the same material was only 45 W/m 2 when it was tested in Colorado on the moist summer day (August 31, relative humidity (RH) = 55%).Mandal et al. 30 manufactured a hierarchically porous polymer radiative cooling coating, which had 96% solar reflectivity and 97% infrared emissivity at 8-13 μm wavelengths.The outdoor experiments showed that the temperature drop of the coating was 6 ℃ under sunlight of 890 W/m 2 in arid Phoenix, while the temperature drop of the coating was only 4. The literature survey indicated that many types of radiative cooling materials had been designed and prepared by researchers.However, practical applications of radiative cooling materials were seriously limited due to the high cost and complexity of preparation.Besides, the literature survey also indicated that the atmospheric water vapor was an important factor affecting the radiative cooling performance.But there was lack of an analysis from the aspect of spectral effective emissivity of the coating.In this work, taking a simple single-layer radiative cooling coating containing two kinds of particle mixture (SiO 2 , TiO 2 ) as example, the spectral effective emissivity of the radiative cooling coating was proposed to evaluate the effect of the atmospheric water vapor on the cooling performance, as shown in Figure 1.The spectral effective emissivity of the coating was obtained through multiplying spectral emissivity of the coating by the atmospheric transmittivity, where the spectral emissivity was calculated by combining an algorithm for calculating radiative properties of the multi-particle system with the Monte Carlo method. Te effects of different atmospheric water vapor on the spectral effective emissivity of coating containing different particles size, volume fraction and thickness were studied.The research results are of great significance to the further application development of radiative cooling materials in different atmospheric water vapor environments.

Theory and methodology
Figure 2 presented the basic procedures to calculate the radiative properties of the coatings by solving the radiative transfer equation (RTE).Firstly, the radiative properties of a single particle were calculated by Mie theory, such as extinction factor, asymmetry factor.Then, the radiative properties of the multi-particle system with non-uniform size were obtained by the algorithm developed by the authors.At last, the spectral reflectivity and emissivity of coatings consisting of base material and multi-particles were obtained by solving the RTE by Monte Carlo ray-tracing method.

Radiative properties of multi-particle system
The multi-particle system was composed of different kinds of particles with different sizes.The radiative properties of a single spherical particle, such as extinction efficiency factor , scattering efficiency factor , scattering phase function ( )   , asymmetry factor g, etc., were governed by two independent parameters: the size parameter and the complex refractive index , where n represented the index of refraction and k represented the index of absorption [33][34][35][36].The spectral complex refractive indexes of TiO 2 and SiO 2 at 0.3-15.0μm wavelength were given in Figure 3 37.The , , ( )   , g and etc. can be calculated by Mie theory [33][34][35][36].
  ext where Re represented the real component of the function, the symbol a n and b n represented the Mie scattering coefficients.The a n and b n were the Mie scattering coefficients. was the scattering angle.The S 1 and S 2 were the complex amplitude functions.The extinction coefficient  , scattering coefficient s  , absorption coefficient  were derived as [33][34][35][36] where n represented the number of the particles, N represented the number density of the particles.The subscript i represented different kinds of particles and the subscript j represented different particle sizes.C e represented the extinction area of the particles and C s represented the scattering area of the particles.The f v represented the volume fraction of the particles.The scattering phase function

 
  of the multi-particle system was modified as: The asymmetry factor g of the multi-particle system was calculated from:

Solving the RTE by MCRT
The multi-particles were embedded in the acrylic resin (base material).The index of refraction of the acrylic resin was 1.5 and the index of absorption of it at 0.3-15.0μm wavelength was much smaller, so it was treated as a non-absorbent medium.The RTE for describing the radiative transfer of the coating containing base material and multi-particle was written as followed and it was solved by using the MCRT method [33][34][35][36]: I  represented the spectral radiative intensity.represented the spectral blackbody intensity.Ω represented the solid angle.The calculated result were the absorptivity, reflectivity and transmissivity of the coating itself.
The basic idea of the Monte Carlo ray tracing method was as following: When a photon bundle traveled in the coating, the bundle would be absorbed and scattered, and the free path length S can be expressed as: The symbol 1  was a random number with a uniform distribution of 0-1.When the photon traveled, another random number 2

Atmospheric total water vapor column (TWC)
There were many factors affecting the atmospheric transitivity ( ), such as H 2 O, O 3 , CO 2 , CO and etc.As shown in Table 1, water vapor had a strong split emission band centered at 1.38, 1.87, 2.7, 6.3 and 71 μm, which affected the atmospheric transmittance in solar waveband and the 'sky window' region 33.The TWC was a method for measuring the total water vapor contained in a vertical column of the atmosphere 39.TWC was relevant to the absolute humidity and local temperature that is not under control.The correlation between the TWC and humidity could be calculated by the empirical table given in MODTRAN, as shown in Table 2.The larger relative humidity, the higher TWC.For example, TWC = 0 atm-cm (RH = 0%), 1000 atm-cm (RH = 10-30%), 3000 atm-cm (RH = 50-60%), 5000 atm-cm (RH = 70-80%), 7000 atm-cm (RH = 90-100%), which included the RH variation in the range of 0-100% 31.

Average effective reflectivity and average effective emissivity
Based on the calculation result of the formula and considering the absorption of the atmospheric water vapor, the effective emissivity of the coating was obtained.The performance of the coating was evaluated according to average effective reflectivity solar R in solar waveband and average effective emissivity  in the 'sky window' region.These two parameters were calculated by 40: I solar represented the solar intensity, R solar represented the spectral reflectance, I BB represented the blackbody radiation intensity.

Model validation
To verify the accuracy of the algorithm developed to calculate the radiative characteristic by the authors, the computed spectral transmittivity was compared with the values gained by the experimental test.The monodisperse SiO 2 standard microspheres (D SiO2 = 284.6 nm) and monodisperse polystyrene (PS) standard microspheres (D PS = 296.5 nm) were selected to compose the multi-particles system for this experiment, where TiO 2 particles were replaced by monodisperse polystyrene standard microspheres due to its inferior monodispersity.SiO 2 and PS standard microsphere solutions were diluted with distilled water to form nanofluids.The volume fractions of SiO 2 and PS standard microspheres in the nanofluids were 0.056% and 0.312%, respectively.A cuvette that optical path length was 1.0 mm was used to keep nanofluids in.
The spectral transmittivity of the nanofluids containing SiO 2 and PS standard microspheres was measured by Ultra-Visible spectrophotometer (TU-1901, Persee, China).According as the effective measuring range of the spectrophotometer was at 400-850 nm wavelengths, the transmittivity of the nanofluids was measured.The related parameters for numerical calculation, such as volume fraction and diameter of the SiO 2 and PS standard microspheres, were based on the above tested values.The complex refractive indexes of SiO 2 , PS and H 2 O were obtained from Ref. 37. The basic procedures to calculate the transmissivity of the nanofluids by solving the RTE had been presented in Figure 2. As shown in Figure 4, the spectral transmittivity of the diluted microsphere solution computed by the algorithm agreed well with the experimental data at all wavelengths.

Effects of TWC on atmospheric transmittivity
In this section, Modtran Demo was used to calculate the atmospheric spectral transmittivity at different TWCs, TWC = 0, 1000, 3000, 5000, 7000 atm-cm.Other calculation parameters were kept unchanged: atmosphere model was mid-latitude summer, ground temperature was set as 301 K, aerosol model was urban, spectral range was 0.3-14.0μm, ozone column value was 0.33176 atm-cm, CO 2 value was 400 ppmv, CO value was 0.15 ppmv, CH 4 value was 1.8 ppmv, the sensor altitude was 50 km 40.
Figure 5 presented the atmospheric spectral transmittivity at different TWCs.As shown in this figure, when the value of TWC was 0 atm-cm, the atmospheric spectral transmittivity was high in both solar waveband and the 'sky window' region.With TWC increasing from 1000 to 7000 atm-cm, the atmospheric spectral transmittivity decreased slightly in solar waveband, while the atmospheric spectral transmittivity decreased significantly in the 'sky window' region.Figure 6 illustrated the atmospheric average transmittivity in solar waveband and "sky window" region at different TWCs., When TWC increased from 0 to 1000 atm-cm, as shown in this figure, the atmospheric average transmissivity in solar waveband dropped rapidly from 75.2% to 64.2% because of the absorption of water vapor.When the values of TWC were 3000, 5000, and 7000 atm-cm, the atmospheric average transmittivity in solar waveband was 59.9%, 57.8%, and 57.2%, respectively.The atmospheric average transmittivity in solar waveband decreased slightly with increasing TWC from 1000 to 7000 atm-cm.In the 'sky window' region, when the value of TWC was 0 atm-cm, the atmospheric average transmittivity was 87.7%.When the values of TWC were 1000, 3000, 5000, and 7000 atm-cm, the average effective transmissivity in the 'sky window' region was 71.2%, 52.0%, 34.1%, and 31.3%, respectively.With the increase of TWC, the atmospheric average transmittivity in the 'sky window' region decreased significantly.It could be concluded from figures that the water vapor had a great influence on the atmospheric average transmittivity, which directly affected the effective emissivity and cooling performance of radiative cooling coatings.Figure 7 presented the comparison of spectral effective emissivity of the coating with/without consideration of the influence of water vapor, TWC = 0 atm-cm and TWC = 3000 atm-cm.Calculating parameters: volume fractions of SiO 2 and TiO 2 particles were kept the same at 3.0%, while diameters of SiO 2 and TiO 2 particles were kept 4 μm and 0.4 μm unchanged, respectively.The coating thickness was 400 μm.As shown in Figure 7, there were certain differences between TWC = 0 atm-cm and TWC = 3000 atm-cm in all calculated spectrum.At 8.0-13.0μm wavelengths, the average effective emissivity of the coating at TWC = 0 atm-cm and TWC = 3000 atm-cm was 79.5% and 48.9%, respectively, with a difference of 30.6%.The atmospheric water vapor had a significant influence on effective emissivity of the coatings, so it could not be ignored in the practical application of the coating.

The effects of particle diameter at different TWCs
In this section, the spectral effective emissivity of the coating with different the diameters of SiO 2 and TiO 2 particles at different TWCs were studied, respectively.The TWCs were 0, 1000, 3000, 5000, 7000 atm-cm.The diameters of SiO 2 particles were 3.0, 4.0, 5.0, 6.0, 7.0 μm, while the diameters of TiO 2 particles were 0.2, 0.3, 0.4, 0.5, 0.6 μm, respectively.In calculation, the volume fractions of SiO 2 particles and TiO 2 particles were kept f v,SiO2 = 2.0% and f v,TiO2 = 2.0% unchanged, while the coating thickness was 300 μm [23,42].Figure 8 presented the influences of diameters of SiO 2 particles on the spectral effective emissivity of the coating at different TWCs, while D TiO2 = 0.4 μm was unchanged.As shown in Figure 8 (a)-(e), as a whole, water vapor had a large influence on the spectral effective emissivity because of its strong absorption in the 'sky window' region.Under the condition of the same diameter of SiO 2 particles, when TWC was within the range of 0-5000 atm-cm, the spectral effective emissivity of the coating decreased sharply with increasing TWC, but the decreasing extent reduced gradually.When TWC was within the range of 5000-7000 atm-cm, the spectral effective emissivity of the coating decreased slowly with increasing TWC.Under the condition of the same TWC, the change trend of the spectral effective emissivity of the coating varied with the diameter of SiO 2 particles was consistent at different TWCs.Taking as an example TWC = 3000 atm-cm, as presented in Figure 8 (c), with increasing the diameter of the SiO 2 particle, the spectral effective emissivity of the coating decreased at 8.0-9.5 μm wavelength, while it increased at 9.5-13.0μm wavelengths.
In order to evaluate the effects of diameters of SiO 2 particles on radiative cooling performance at different TWCs, the average effective emissivity of the coating at 8.0-13.0μm wavelengths was calculated and the results were shown in Figure 9.With increasing the diameter of SiO 2 particles, the average effective emissivity of the coating increased first and then decreased at different TWCs.When the SiO 2 particle size was 4.0 μm, the average effective emissivity of the coating at 8.0-13.0wavelengths reached the highest value.The highest emissivity at this particle size was mainly because resonance occurred to excite higher-order electric magnetic modes in the 'atmospheric window' spectrum.Besides, the average effective emissivity of the coating decreased with increasing the TWC.Taking for example the D SiO2 = 4.0 μm, the average effective emissivity in the 'sky window' region was 74.8% when the value of TWC was 0 atm-cm.The average effective emissivity of the coating at 1000, 3000, 5000 and 7000 atm-cm was 62.0%, 45.8%, 32.8%, 31.6%,respectively, with a decrease of 12.8%, 29.0%, 42.0%, 43.2%.It seriously affected the ability of the coating to emit energy to outer space, which resulted in that cooling effect was not observed in high humidity areas.Figure 10 presented the effects of diameters of TiO 2 particles on the spectral effective emissivity of the coating at different TWCs.Compared Figures 8 and 10, it can be seen that the TiO 2 particle had little influence on the spectral effective emissivity at 8-13 μm wavelengths, but affected the spectral emissivity in solar waveband (0.3-2.5 μm).As presented in Figure 10(a),(b), under the condition of the same diameter of TiO 2 particles, when TWC increased from 0 to 1000 atm-cm, the spectral effective emissivity of the coating decreased obviously because the absorption peaks of the water vapor in solar waveband were 1.38 μm and 1.87 μm.However, when TWC was within the range of 1000-7000 atm-cm, the spectral effective emissivity of the coating showed minor changes with variation of TWC.As presented in Figure 10 (c), taking as an example TWC = 3000 atm-cm, the spectral effective emissivity oscillated with the change of wavelength.This phenomenon was induced due to the reason that TiO 2 particle size was in the strong Mie scattering region at 0.3-0.8μm wavelengths.With increasing the diameter of TiO 2 particles, the spectral effective emissivity decreased at 0.3-0.8μm wavelengths, while it increased at 0.8-2.5 μm wavelengths.
The influences of diameters of TiO 2 on the average effective reflectivity (1-absorptivity-transmissivity) of the coating at different TWCs were shown in Figure 11.The average effective reflectivity of the coating first increased and then decreased at different TWCs with increasing the diameter of TiO 2 particles.When the TiO 2 particle size was 0.4 μm, that average effective reflectivity of the at all different TWCs can reach the highest value.This was mostly because the TiO 2 with this average particle size was equivalent to the incident wavelength of the sun, which could exert a strong Mie scattering effect.Although the average effective reflectivity of the coating in solar waveband decreased gradually with the increase of TWC, this did not directly affect the cooling performance of the coating because there was no heat exchange process.

The effects of particle volume fraction at different TWCs
The effects of the volume fraction of SiO 2 and TiO 2 particles on the spectral effective emissivity of the coating at different TWCs were investigated.The TWCs were 0, 1000, 3000, 5000 and 7000 atm-cm, respectively.The volume fractions of both SiO 2 and TiO 2 particles were 0.5%, 1.0%, 2.0%, 3.0%, 4.0%.The diameters of SiO 2 particles and TiO 2 particles were kept D SiO2 = 4 μm and D TiO2 = 0.4 μm unchanged, while the coating thickness was 300 μm.
Figure 12 showed that the influences of volume fraction of SiO 2 and TiO 2 particles on the spectral effective emissivity of the coating at different TWCs.Under the condition of a certain TWC, the effect of the volume fraction of the SiO 2 and TiO 2 particles on the spectral effective emissivity of the coating in different waveband was different.When the wavelength was in 0.3-2.5 μm wavelengths, with increasing the volume fraction of SiO 2 and TiO 2 particles, the spectral effective emissivity of the coating decreased firstly and then remained unchanged.On the contrary, when the wavelength was in 8.0-13.0μm wavelengths, the spectral effective emissivity increased firstly with the increase of the volume fraction of SiO 2 and TiO 2 particles, and it reached a stable state when the volume fraction of SiO 2 and TiO 2 particles was 3.0%.Under the condition of a certain volume fraction of SiO 2 and TiO 2 particles, with increasing TWC from 0 to 7000 atm-cm, the spectral effective emissivity of the coating decreased significantly.Besides, strong absorption of water vapor weakened the influences of particle volume fractions on the spectral effective emissivity of the coating.Figure 13 presented that the influences of volume fraction of SiO 2 and TiO 2 particles on the average effective emissivity of the coating at different TWCs.As shown in this figure, increasing TWC from 0 to 5000 atm-cm, the average effective emissivity of the coating decreased substantially.The average effective emissivity decreased slightly with increasing TWC when it was in the range of 5000-7000 atm-cm.The average effective emissivity increased first with increasing volume fraction of SiO 2 and TiO 2 particles, and it basically remained unchanged when the volume fraction went up to 3.0%.The main reason for this phenomenon was that the blocking effect of the particles in the coating increased with increasing volume fraction of SiO 2 and TiO 2 particles.Taking the f v,SiO2 = 3.0% for example, the average effective emissivity of the coating in the "sky window" region was 75.8% when the value of TWC was 0 atm-cm.The average effective emissivity of the coating at 1000, 3000, 5000 and 7000 atm-cm was 62.9%, 46.6%, 33.1%, 31.9%,respectively, with a relative decrease of 12.9%, 29.2%, 42.7%, 43.9%.

The effects of coating thickness at different TWCs
In this section, the effects of the coating thicknesses on the spectral effective emissivity of the coating at different TWCs were studied.The TWCs were 0, 1000, 3000, 5000 and 7000 atm-cm, respectively.The coating thicknesses were 250, 300, 350, 400, 450, 500 μm, respectively.The diameters and volume fractions of SiO 2 and TiO 2 particles were the optimal values based on the above calculations.
Figure 14 presented that the influences of coating thicknesses on the spectral effective emissivity of the coating at different TWCs.As shown in Figure 14 (a), when the value of TWC was 0 atm-cm, with the increase of coating thicknesses, the spectral effective emissivity of the coating remained unchanged at 0.3-1.0μm wavelengths, while it decreased gradually and then basically remained unchanged at 1.0-2.5 μm wavelengths.When TWC was in the range of 1000-7000 atm-cm, it could be seen from Figure 14 (b)-(e) that the spectral effective emissivity of the coating decreased gradually with increasing coating thickness in overall solar waveband.Under Figure 15 presented that the influences of coating thicknesses on the average effective emissivity of the coating at different TWCs.As shown in this figure, under the condition of the different TWCs, the average effective emissivity of the coating increased first and remained unchanged with the increase of the coating thickness.Taking as an example TWC = 1000 atm-cm, when the coating thickness increased from 250 μm to 400 μm, the average effective emissivity of the coating increased from 60.1% to 66.7%, with an increase of 6.6%.However, with the thickness increased from 400 μm to 500 μm, the average effective emissivity of the coating increased from 66.7% to 67.0%,only increased by 0.3%.As the thickness of the coating increased, the blocking effect of the particles in the coating became more obvious so that the average effective emissivity would not show a high growth rate with increasing coating thickness.When the thickness of the coting was 400 μm, the average effective emissivity of the coating decreased from 79.5% to 35.3% with increasing TWC from 0 to 7000 atm-cm, with a decrease of 44.2%.

Conclusions
In this study, taking a simple single-layer radiative cooling coating containing two kinds of particle mixture (SiO 2 , TiO 2 ) as example, the spectral effective emissivity of the radiative cooling coating was proposed to evaluate the effect of the atmospheric water vapor on the cooling performance.The effects of different atmospheric water vapor on the spectral effective emissivity of coating containing different particles size, volume fraction and thickness were studied.Results showed that the influences of the volume fraction of particles and coating thickness on the average spectral effective emissivity were getting weak with the increase of TWC and these two parameters decreased properly.With consideration of the atmospheric water vapor, the simple single-layer radiative cooling coating filled with 5.0% of TiO 2 particles with a diameter of 0.4 μm and 5.5% of SiO 2 with a diameter of 4 μm can obtain the best spectral effective emissivity.Based on the above calculation parameters, with increasing TWC from 0 to 7000 atm-cm, the average effective emissivity of the coating decreased from 79.5% to 35.3%, with a decrease of 44.2%.This work is of great significance to the further application development and the design criterion of radiative cooling materials in different atmospheric water vapor environments.
5 ℃ under sunlight of 760 W/m 2 in coastal New York.Liu et al. 31 demonstrated a hierarchical porous cooling material having a solar reflectivity of 95% and long-wave emissivity of 95%.The temperature drop in dry season could reach 6 ℃, while it was only 2.7 ℃ in the humid season.Li et al. 32 did an detailed analysis of the contribution of atmospheric constituents (including water vapor) to the spectral values of the sky emissivity, and proposed correlations for the effective sky emissivity in several longwave bands as functions of the normalized ambient partial pressure of water vapor.

Figure 1 .
Figure 1.Schematic diagram of the influences of TWCs on cooling performance of the coating.

Figure 2 .
Figure 2. Basic procedures of the algorithm to calculate the optical properties of the coatings by solving the RTE.

Figure 3 .
Figure 3.The complex refractive indexes of SiO 2 and TiO 2 .

2 . If 2 
to determine whether the photon was to be absorbed or scattered.The random number was compared with the scattering albedo    >  , the photon would be absorbed, otherwise the photon would be scattered.For more details about the MCRT, please refer to the papers 38.b I 

Figure 4 .
Figure 4. Comparisons of the spectral transmittivity between tested values and calculated results.

Figure 6 .
Figure 6.The average transmittivity of the atmosphere in solar waveband and 'sky window' region at different TWCs.

Figure 7 .
Figure 7. Comparisons of spectral effective emissivity of the coating between the TWC = 0 atm-cm and TWC = 3000 atm-cm.

Figure 8 .
Figure 8. Effects of diameters of SiO 2 particles on spectral effective emissivity at different TWCs.

Figure 9 .
Figure 9. Effects of diameters of SiO 2 particles on the average effective emissivity at different TWCs.

Figure 10 .
Figure 10.Effects of diameters of TiO 2 particles on the average effective emissivity at different TWCs.

Figure 11 .
Figure 11.Effects of diameters of TiO 2 particles on the average effective reflectivity of the coating at different TWCs.

Figure 12 .
Figure 12.Effects of volume fraction of SiO 2 and TiO 2 particles on the spectral effective emissivity at different TWCs.

Figure 13 .
Figure 13.Effects of volume fraction of SiO 2 and TiO 2 particles on the average effective emissivity at different TWCs.

Figure 15 .
Figure 15.Effects of coating thickness on the average effective emissivity at different TWCs.

Table 1 .
Split emission band center of water vapor 33.

Table 2 .
The calculated ground absolute humidity and TWC for the typical atmospheric model in MODTRAN (2018) 27.